#------------------------------------------------------------------------------
#$Date: 2024-05-09 10:47:05 +0200 (Thu 09 de May de 2024) $
#$Revision: 291792 $
#$URL: svn://www.crystallography.net/cod/cif/9/01/13/9011355.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9011355
loop_
_publ_author_name
'Hassan, I.'
'Peterson, R. C.'
'Grundy, H. D.'
_publ_section_title
;
 The structure of lazurite, ideally Na6Ca2(Al6Si6O24)S2, a member of the
 sodalite group
;
_journal_name_full               'Acta Crystallographica, Section C'
_journal_page_first              827
_journal_page_last               832
_journal_paper_doi               10.1107/S0108270185005662
_journal_volume                  41
_journal_year                    1985
_chemical_compound_source        'Sary-Sang, Afghanistan'
_chemical_formula_sum            'Al2.97 Ca0.8 Mg0.36 Na3.12 O15.12 S Si3.03'
_chemical_name_mineral           Lazurite
_space_group_IT_number           218
_symmetry_space_group_name_Hall  'P -4n 2 3'
_symmetry_space_group_name_H-M   'P -4 3 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   9.105
_cell_length_b                   9.105
_cell_length_c                   9.105
_cell_formula_units_Z            2
_cell_volume                     754.814
_database_code_amcsd             0010009
_exptl_crystal_density_diffrn    2.428
_cod_original_formula_sum        'Na3.12 Ca.8 Mg.36 Al2.97 Si3.03 O15.12 S'
_cod_database_code               9011355
loop_
_space_group_symop_operation_xyz
x,y,z
-z,x,-y
-y,z,-x
-x,y,-z
1/2+x,1/2-z,1/2-y
1/2+z,1/2-y,1/2-x
1/2+y,1/2-x,1/2-z
1/2+x,1/2+z,1/2+y
1/2+z,1/2+y,1/2+x
1/2+y,1/2+x,1/2+z
-z,-x,y
-y,-z,x
-x,-y,z
z,-x,-y
y,-z,-x
x,-y,-z
1/2-x,1/2+z,1/2-y
1/2-z,1/2+y,1/2-x
1/2-y,1/2+x,1/2-z
1/2-x,1/2-z,1/2+y
1/2-z,1/2-y,1/2+x
1/2-y,1/2-x,1/2+z
z,x,y
y,z,x
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
Na1 0.17800 0.17800 0.17800 0.35000 0.05200
Na2 0.23100 0.23100 0.23100 0.21000 0.04100
Ca2 0.23100 0.23100 0.23100 0.20000 0.04100
Mg2 0.23100 0.23100 0.23100 0.09000 0.04100
Na3 0.30500 0.30500 0.30500 0.22000 0.03500
Al 0.25000 0.00000 0.50000 0.99000 0.03400
Si 0.25000 0.00000 0.50000 0.01000 0.03400
Si 0.25000 0.50000 0.00000 1.00000 0.03900
O1 0.13300 0.14700 0.54500 0.50000 0.03900
O2 0.15700 0.15800 0.47400 0.50000 0.03900
O3 0.59800 0.59800 0.59800 0.78000 0.21200
S 0.00000 0.00000 0.00000 1.00000 0.16800
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0010009
